Statistical optimization of experimental parameters for extracellular synthesis of zinc oxide nanoparticles by a novel haloalaliphilic Alkalibacillus sp.W7

Green synthesis of zinc oxide nanoparticles (ZnO NPs) through simple, rapid, eco-friendly and an economical method with a new haloalkaliphilic bacterial strain (Alkalibacillus sp. W7) was investigated. Response surface methodology (RSM) based on Box-Behnken design (BP) was used to optimize the process parameters (ZnSO4.7H2O concentration, temperature, and pH) affecting the size of Alkalibacillus-ZnO NPs (Alk-ZnO NPs). The synthesized nanoparticles were characterized using UV–visible spectrum, X-ray diffraction (XRD), Scanning electron microscope-energy dispersive X-ray spectroscopy (SEM–EDX), Transmission electron microscopy (TEM), Fourier transform infrared spectroscopy (FTIR) and Zeta potential. The UV–Vis spectrum of ZnO NPs revealed a characteristic surface plasmon resonance (SPR) peak at 310 nm. XRD pattern confirmed the hexagonal wurtzite structure of highly pure with a crystallite size 19.5 nm. TEM proved the quasi-spherical shape nanoparticles of size ranging from 1 to 30 nm. SEM–EDX showed spherical shaped and displayed a maximum elemental distribution of zinc and oxygen. FTIR provided an evidence that the biofunctional groups of metabolites in Alkalibacillus sp.W7 supernatant acted as viable reducing, capping and stabilizing agents.

Nanoparticles (NPs) with at least one dimension sized from 1 to 100 nm 1 exhibit unique features owing to their extremely small size and high surface area to volume ratio, which have attributed to the significant differences in the properties over their bulk counterparts 1,2 . The increasing research in the field of nanotechnology has influenced many areas such as energy, medicine, electronics, environment, catalysts and space industries [3][4][5] .
The synthesis of nanoparticles with the help of microorganisms has no harmful impacts, does not require use of hazardous chemicals, energy efficient, simple, clean, economical, and provides greater biocompatibility especially in the clinical and biomedical applications 6 . In addition the various natural materials in microorganisms function as a potential biofactory for the reduction and stabilization of the nanoparticles 7,8 . Moreover, simple downstream processing provides greater biocompatibility in the uses of nanoparticles for pharmaceutical and biomedical applications and effective sources for high productivity and purity 9,10 . One of the few disadvantages for microbial synthesis of nanoparticles is the tedious purification steps and poor understanding of the mechanisms controlling the shape, size, and mono dispersity.Also, scaling up the production processing for industrial applications is a challenge for its commercialization. Another challenge is slection of biocatalyst and optimization of reaction condition to achieve better yield and small size 9,10 .
Zinc oxide nanoparticles (ZnO NPs) are one of the most important metal oxide with many significant features such as chemical and physical stability, high catalytic activity, effective antibacterial activity as well as intensive ultraviolet (UV) and infrared (IR) adsorption 11 . They are used in an array of products and wide range of applications 1,12,13 .
Traditionally, ZnO NPs synthesized by various physicochemical methods suffer from drawbacks such as high cost, requirement of elevated temperature, high pressure, specialized equipment, use of toxic and environmentally hazardous chemicals; resulting in high energy consumption and the generation of large amounts of waste which

Results and discussion
Extracellular synthesis of Alk-ZnO NPs. To the best of our knowledge, this is the first report employing Alkalibacillus sp. W7 as a natural nanofactory for extracellular synthesis of ZnO NPs. The preliminary detection of nanoparticles formation was distinguished through visual observation of cloudy white clusters deposited at the bottom of the tube compared to control (Fig. 1). The cloudy white precipitate arised as a result of reduction of Zn +2 ions to elemental Zn 0 by active metabolites in the culture filtrate and is due to the excitation of surface plasmon resonance (SPR) of the ZnO nanoparticles 24 . It has been demonstrated that the proteins, enzymes as well as other active metabolites secreted by microorganisms are the principal biomolecules involved in the formation of metal/metal oxide nanoparticles 4,25 . It was found that the UV-vis absorption spectrum of biosyn-   Table 1. It was observed that the smallest sized particles were produced from trials 2, 4, and 12. The determination coefficient (R 2 ) values provide a measure of how much variability in the observed response can be explained by the experimental factors and their interactions. The closer the R 2 value to 1, the stronger the model is, the better it predicts the response and has a very high correlation 22,27 . The determination coefficient (R 2 ) of the model (0.9654) indicates 96.54% of variability in the response. Therefore, the present R 2 -value indicates a very good fit between the observed and predicted responses and implies that the model is reliable in the present study.
Analysis of variance (ANOVA) was used to evaluate the significance and adequacy of the regression model. According to ANOVA results (Table 2), the model was highly appropriate; the relationship between the independent variables and the average size of nanoparticles was evident from low P-value (0.00378).
The value of adjusted-R 2 (0.9033) was also very high indicating a high significance of the model 22 and suggested that the total variation of 90.33% average diameter size of nanoparticles is attributed to the independent variables and only about 9.67% of the total variation cannot be explained by the model. All values of model coefficients were calculated by multiple regression analysis. The significance of each coefficient was determined by the Student's t-test and P-value, as illustrated in Table 3. Based on the analysis of regression coefficients of the quadratic model, among the three tested variables, the linear effects of reaction pH (X 1 ), and reaction temperature (X 2 ) exhibited a negative relationship on particle size, while zinc sulphate concentration (X 3 ) exhibited a positive relationship. P-value indicates the significance of each of the coefficients which is important to understand the pattern of the mutual interaction among variables. The smaller the magnitude of the P, the more significant is the corresponding coefficient. According to the degree of significance (P ≤ 0.01, significant at 99% level), the linear term of pH (X 1 ) had the most dramatic negative significant effect on NPs size among all linear effects. In contrast, the www.nature.com/scientificreports/ quadratic terms for pH (X 1 2 ), temperature (X 2 2 ) and metal concentration (X 3 2 ) had a significant positive effect; meaning that they could be considered as limiting factors and little variation in their values will alter the size of nanoparticles. In addition, only interaction between pH (X 1 ) and metal concentration (X 3 ) was noted to have a negative significant effect.
The Pareto chart identified as a useful tool for determining the most significant effects 28 was used to illustrate the order of significance of the different factors on Alk-ZnO NPs size. Each bar length on a standardized Pareto chart (Fig. 2) is proportional to the absolute value of its related estimated effect or regression coefficient.
Design Expert software was used to fit a second order polynomial model to the experimental results to predict the size of NPs within the experimental constraints. The following second order polynomial equation represents the empirical relationship between NP size and the three independent variables: The coefficients sign determines the response performance. Here, coefficient with positive effect means decrease in particle size, while a negative effect means increase in particle size. In addition, at higher absolute value of a coefficient, the effect of variable is higher. Therefore, according to the previous equation, pH of the reaction is the variable with the strongest influence on NPs size. www.nature.com/scientificreports/ From polynomial models, response surface curves were plotted using Design-Expert 7.0, a trial version software to determine the effects of factors and their combinations that optimize the response. These threedimensional plots and their respective contour plots provided a visual interpretation of the interaction of two test variables with the third one held at a constant level and facilitated the location of optimum values of the variables for synthesis of the smallest NPs. Significance of the interaction plots between the corresponding variables was indicated by an elliptical or circular or saddle nature of the contour plots 23 . The contour plots ( Fig. 3) reveal that the optimal point for decreasing the average diameter of Alk-ZnO NPs was located inside the experimental region, which confirms the adequacy of the independent variable concentration ranges used in this study. The response surfaces obtained were concave, indicating that the operating conditions were well-defined and optimum. Figure 3A represents the interaction between temperature and metal concentration and reveals that the average diameter size decreased with gradual increasing in both metal concentration and temperature. This might be explained that increasing metal ion concentration to a certain point allows particle growth at a faster rate and generates NPs with smaller size. Moreover, higher metal precursor concentration in the reaction mixture may increase the aggregation of the growing NPs, which resulted in the formation of larger NPs size 21,29 . Phanjom &Ahmed 30 reported that AgNO 3 concentration up to 8 mM, resulted in the formation of a smaller nanoparticle size, while the size increased at 9 and 10 mM concentrations. This effect was attributed to the lack of functional groups available for the reaction when the metal precursor concentration was increased. To achieve the smallest particle size, the middle levels of both metal concentration and temperature were used. Higher temperature resulted in the gradual increase in the NPs size. Unsuitable temperatures lead to increased nanoparticle size and loss of stability, as a result of denaturation, inactivation or low activity of the reductive enzymes and other active molecules involved in the biogenesis process 31,32 . Additionally, it was suggested that the increase in temperature decreases NPs size which is normally due to increment in reaction rate and kinetic energy at higher temperatures 29,33 . Generally, the effect of temperature on the size and stability of the synthesized nanoparticles varies according to the microorganism used 9 . Figure 3B represents the mutual interaction of pH and metal concentration on Alk-ZnO NPs biosynthesis when temperature was fixed at optimum value. The average diameter size decreased gradually with the increment of pH but at higher pH values, the size slightly increased. This may be due to the inactivation of biomolecules involved in the synthesis of Alk-ZnO NPs at low and high pHs 21 . Generally, pH plays a significant role in nanoparticles synthesis, mainly because it has the ability to alter the shape of biomolecules that is responsible in capping and stabilizing the NPs 34 . Also, plays a www.nature.com/scientificreports/ substantial role in the oxidation state and reducing power of enzymes and secondary metabolites present in cell-free extract 35 . Zhang et al. 36 stated that pH of the medium solution influences the size and the texture of the synthesized nanoparticles. Modification in pH leads to alteration in the overall charge of bioactive molecules, which in turn facilitates their binding affinity and hence biomineralization of metal ions into nanoparticles 37 . The obtained data reveal that alkaline pH and a high metal concentration are conditions that will generate smallest size of Alk-ZnO NPs. While, a higher or lower pH generated the larger size, which indicated that the catalytic activity of enzymes responsible for Zn 2+ ions reduction appeared to be deactivated, thus causing an increase in the size of NPs. Figure 3C shows the combined effect of pH and temperature when metal concentration value was fixed at optimum value. It showed that higher values of pH and temperature supported the increase of Alk-ZnO NPs size. The smallest size was obtained in the middle levels of both pH and temperature. The synthesis of small sized ZnO NPs could be attributed to the increase in nucleation process rate as a result of a large number of OH ions. The finding is in agreement with that reported by Mata et al. 38 who indicated that higher pH favored higher reducing power. Possible reason is that during the elevated pH, the reaction rate will be increased with subsequent crystallization into smaller particles, which involved the nucleation and growth processes of smaller particles from metal nuclei 39 .
The study of physicochemical parameters of the reaction such metal ions concentrations, pH and temperature on Alk-ZnO NPs formation represents the effect of the direct connection between these factors on the particles size. By solving the model regression equation using the SOLVER function of MICROSOFT EXCEL tools, the smallest size Alk-ZnO NPs and the optimum values of these variables can be acquired. The optimal values of the variables were temperature 33 °C, metal concentration 8 mM and pH 8. The model predicts the smallest NPs size that can be obtained using the above optimum conditions to be 20.4 nm. Verification of the model. In order to validate the obtained data and to evaluate the accuracy of the applied Box-Behnken statistical design, a verification experiment with optimum concentration of examined variables was carried out in three replicate and compared with the predicted data. The results obtained demonstrated that the average size of nanoparticles was 17.5 nm, while the predicted value from the polynomial model was 20.4 nm. There was a little difference between the experimental and the predicted data. The verification revealed a high degree of accuracy of the model, indicating the model validation under the tested conditions. The measured particle size was less than the predicted by 14.22%. Verification experiment indicated validity, and reliability of response model and applicability of RSM to minimize the size of Alk-ZnO NPs. Additionally, in the present study, Al. sp.W7 could synthesize 0.493 g of NPs /L of bacterial supernatant in 24 h.

Characterization of Alk-ZnO NPs. UV-visible spectroscopy. Alk-ZnO NPs synthesized under optimal
conditions exhibited the surface plasmon resonance band shifted to a lower wavelength 310 nm, due to their large excitation binding energy 40 . It is known from absorption spectroscopy that as particle size decreases, the band gap energy increases. There is also an opposite ratio between band gap and the absorption wavelength 41 . The corresponding band gap was found to be 4.00 eV. Our data are in good agreement with the earlier reports on biosynthesis of ZnO NPs 25,42 . Aggregation is a common problem with nanoparticles which greatly decreases the surface area and, as a result, affects their physicochemical and biological properties 43 . It is worth to mention that the nanoparticles examined after 10 months using UV-vis spectroscopy showed a peak at 310 nm, indicating their stability (Supplementary Figure S1).
Scanning electron microscopy analysis. Scanning electron microscopy provided further insight into the morphology and size of the synthesized ZnO NPs. The micrograph illustrated in Fig. 4 proved that they had nanosized range, smooth, irregular to nearly spherical with a uniform distribution with an average size ranging from 5 to 45 nm. www.nature.com/scientificreports/ Energy-dispersive X-ray spectrum. The Alk-ZnO NPs were subjected to an EDX spectrum to quantify the mixture of metal and oxides present in the sample. Figure 5 clearly illustrates that the EDX spectrum of the fabricated NPs was recorded in the spot-profile mode from one of the densely populated nanoparticles area. Distinct peaks obtained for zinc and oxygen atoms represent the formation of ZnO NPs. The elemental profile showed strong higher peak at 1 keV, characteristic to Zn and confirmed the formation of ZnO NPs 44,45 . The weak signal of C atoms was also recorded and likely due to X-ray emission from carbohydrates/proteins/enzymes present in the bacterial cell free filtrate indicating their involvement in reduction and capping of the synthesized ZnO NPs. The atomic percentages of the elements inset of Fig. 5 reveal zinc as the major element comprising more than 66.33% of total constituent along with oxygen 25.48%, which clearly also confirms the high purity of mediated zinc oxide nanoparticles. Additionally, the optical absorption signals of zinc were observed due to surface plasmon resonance of ZnO NPs 34,45 , which is in agreement with previous reports 46,47 . The impurity free nanoparticles are promising in different application fields as antitumor, anti-microbial and antibiofilm. Our results are in agreement with the results obtained by microbially synthesized ZnO NPs 20,47,48 , where pure form of nanoparticle was clearly depicted through EDX imaging.
Transmission electron microscopy. Transmission electron microscopic analysis provided exact morphology and size of Alk-ZnO NPs acquired from optimized synthesis conditions and revealed predominantly irregular to nearly hexagonal and quasi-spherical with legitimately agglomeration (Fig. 6A,B). This is a typical phenomenon of interaction of moisture and ZnO and inter-particle interactions (Van der Waals, electrostatic and magnetic forces) 49,50 . The size distribution patterns reveal that the synthesized NPs ranged from 1-30 nm with an average size of 17 ± 1 nm (Fig. 6C). This result is in accordance with crystallite size calculated from the X-ray diffraction. Similar hexagonal-quasi-spherical zinc oxide nanoparticles have been observed in Rhodococcus pyridinivorans NT2 46 and Lactobacillus plantarum VITES07 51 . It was previously reported that the smaller the size of ZnO NPs, the greater efficacy in inhibiting the growth of bacteria 52 .  (Fig. 7). The XRD diffraction peaks were in good agreement with the reported literature and matched well with wurtzite ZnO of the Joint Committee on Powder Diffraction Standards (JCPDS) Card number 36-1451. Thus XRD pattern shows ZnO NPs with a fine hexagonal crystalline structure formed with significant agreement with this reference file, and no characteristic diffraction peaks were observed other than ZnO, indicating that the bio-assisted NPs were free from other phase impurities and significantly had a high phase purity 13,53 , which was confirmed by EDX analysis results. In addition, the strong and narrow diffraction peaks indicated that the ZnO nanoparticles were of well crystalline structure 46 . Our results are in good agreement with various XRD diffractogram data reported for biologically synthesized ZnO nanoparticles 24,46 . The average crystalline size of NPs corresponding to the most intense diffraction peak at 2θ = 35.65 o (101) as calculated by Debye-Scherrer′s equation was found to be 19.5 nm. XRD results confirmed that Alk-ZnO NPs are highly crystalline, having hexagonal wurtzite crystalline structure which are compatible with other researchers' work 20,55 . XRD results also reflect that the crystallization of the bio-organic phase occurs on the surface of the ZnO NPs. The biosynthesized ZnO nanoparticles shared accord with the crystallite size calculated from TEM.  www.nature.com/scientificreports/ Zeta potential. Zeta potential of the suspension is one of the key parameters in assessing the stability of the synthesized nanoparticle as it gives the net electrostatic potential of any particle in suspension. The biosynthesized zinc oxide nanoparticles possessed a high positive potential value of 27.5 mv (Fig. 8) which indicates that they were highly stable and prevented agglomeration due to strong electrostatic repulsive forces between them. Nanoparticles with high negative or positive Zeta potential never aggregate due to electrostatic force of repulsion while particles with low zeta potential tend to flocculate 51 . It is generally considered that the zeta potential values (+ 30 mV to − 30 mV) result in good nanoparticle stability 17,51 , this result is comparable with zeta potential of zinc nanoparticles synthesized by Pseudomonas hibiscicola (24.64 mV) 24 . Positively charged nanoparticles show better attachment towards negatively charged cell membrane surface due to electrostatic attraction which leads to the penetration of ZnO NPs into the cells and thus enhanced toxicity towards microorganism 56 .

X-ray diffraction analysis. X-ray diffraction is taken in order to further confirm
Fourier transform infrared. FTIR spectrum was performed to determine the surface chemistry of the ZnO NPs and is used to access the details of functional groups involved in the biomolecules responsible for reducing and capping the bio-reduced ZnO NPs 25,57 . The FTIR spectra for ZnO NPs are presented in Fig. 9. The broad stretching vibrational band with high intensity observed at 3369 cm -1 is characteristic for hydroxyl group (OH) or can correspond to the protein N-H amide I 51 . It is well known that protein-nanoparticle interactions can occur either through free amine groups or cysteine residues in proteins and via the electrostatic attraction of negatively charged carboxylate groups in enzymes 53 . The absorption peak at 2922 cm −1 is attributed to C-H stretch of the methylene groups of the protein stretching 21 . Bands at 2352 and 2109 cm −1 are associated with the presence of primary amines and sulfur compounds 44 . These peaks indicate the presence of proteins and other organic residues, which might have produced extracellularly by Al.sp. W7. Moreover, the absorption peak at   59 . According to Tiwari et al. 60 , metal oxides exhibit absorption bands well below 1200 cm −1 arising due to interatomic vibrations. Generally metal oxides give absorption peaks in the regions between 500 and 900 cm −154 . Strong peaks observed at 578.95 cm −1 and 906 cm −1 prominently indicate Zn-O bond. These findings are in accordance with literature values 20,41 . The stretching mode peaks are indicative of the successful synthesis of ZnO nanoparticles from Al.sp. W7 and FTIR spectral analysis reveals the subtle variations in biological components of culture supernatant associated with ZnO NPs formed. The functional groups present in secreted proteins, enzymes and secondary metabolites in strain W7 culture supernatant are responsible for reduction of metal ions and biosynthesis of metallic nanoparticles. The significant reduction capabilities of the biofunctional groups (R-OH, R-NH 2 , R-COO − ) would reduce Zn 2+ as electron acceptor to Zn 0 resulting in the formation of ZnO NPs. These metabolites not only act as reducing agents but also act as capping agents providing stabilization against aggregation. These results are in agreement with previous report in green ZnO NPs synthesis 13,61 . Alkalibacillus sp. W7 nanoparticles showed good antibacterial activity, inhibiting the growth of Gram-negative and Gram-positive bacteria and also efficient photocatalytic degradation of the methylene blue and methyl orange dye under solar irradiation 62 . Moreover, biofilm inhibition activity, anticancer and antioxidant potentials of the synthesized nanoparticles were also investigated.

Materials and methods
Microorganism and cultural conditions. Alkalibacillus sp. W7 an aerobic Gram-positive, rod-shaped bacterium, isolated from hypersaline Lake Al-Hamra in Wadi An-Natrun, Egypt was used in this study. The 16S rDNA sequence was submitted to NCBI GenBank with an assigned accession number LC164829 63 . The strain was maintained on modified Horikoshi-I medium 64  The color change was observed in the reaction mixture due to the reduction reaction. Simultaneously, control of sterile uninoculated media mixed with precursor salt solution was also maintained at same condition along with the experimental tubes in triplicate.

Statistical optimization of ZnO nanoparticles biosynthesis. Response surface methodology (RSM)
is a collection of mathematical and statistical techniques which has been known as a tool for modeling within minimum number of experimental runs, determining the effects of important parameters and to identify their prominent interactions for the best response 21,23 .
Response surface methodology based on Box-Behnken design 27 was used to evaluate the relationship between the factors that optimize the response. The combined effect of three active independent variables; pH (X 1 ), reaction temperature (X 2 ) and Zinc sulphate concentration (X 3 ) was considered for evaluation. Their effects were evaluated with respect to responce (NPs size). The levels of each individual variable were selected based on the results of preliminary experiments, involving optimization using the one-factor-at-a-time method. Table 1 shows the experimental Box-Behnken design matrix in the coded and actual levels of selected independent variables developed by Design Expert software (Version 7, Stat-Ease, Inc., USA) and the responce. Statistical analysis. Hence, for a three-variable design, a total of 15 experimental runs were performed and their observations were fitted in the second order polynomial model, which is a mathematical expression used to determine the linear, quadratic, and cross effects of the tested independent variables to find the result and approximate the real answer as follows: where Y is the dependent variable (size of NPs), X 1 , X 2 , and X 3 are the independent variables, β0 is the regression coefficient at center point, β 1 , β 2 , and β 3 are the linear coefficient; β12, β13, and β23 are the second order interaction coefficients, and β11, β22, and β33 are the quadratic coefficients.
Purification of Alk-ZnO NPs. The nanoparticles were separated from the reaction mixture by high-speed centrifugation at 15,000 rpm for 10 min, then dispersed in sterilized distilled water and centrifuged again. This action was carried out for three times to remove the unreacted metals and the residual biological molecule impurities or any residual metabolites from native nanoparticle samples to obtain purified NPs 6 . Finally, the obtained Y = β 0 + β 1 x 1 + β 2 x 2 + β 3 x 3 + β 12 x 1 x 2 + β 13 x 1 x 3 + β 23 x 2 x 3 + β 11  Characterization of biogenic ZnO NPs. UV-visible spectroscopy. The biosynthesized ZnO NPs were characterized using UV-Vis spectrophotometer (Thermo Scientific Evolution TM 300) in the wavelength region between 200-nm and 900-nm operated at a resolution of 1 nm and maximum absorbance was determined 65 .
X-ray diffraction. X-ray diffraction was performed using Phaser XRD-D2 powder X-ray diffractometer (Bruker, Germany) supplied with Cu-Kα radiation over a wide range of the Bragg angles θ (10° ≤ 2θ ≤ 80°) operated at 30 kV, 10 mA. Data was compared with known standard data published by the Joint Committee on Powder Diffraction Standards (JCPDS Card No. . The mean of the crystallite size (nm) was determined from the XRD line broadening measurement using Debye Scherrerr's equation: where λ is the wavelength of X-ray radiation, λ = 1.5406 Å, β is the full width at the half maximum (FWHM) of the most intense diffraction peak, and θ is the diffraction angle.
Scanning electron microscopy. The shape and size of the ZnO NPs were determined using SEM JEOL IT 200, (JOEL Corp, Tokyo, Japan). The biosynthesized powder was mixed into doubled distilled water and sonicated for 30 min. A small drop of this sample was allowed to dry on a glass slide to make a thin layer of NPs.
Energy-dispersive X-ray analysis. The structure of Alk-ZnO NPs was characterized by energy-dispersive analysis X-ray (EDX) spectrum using X-ray micro-analyzer (Module Oxford 6587INCA X-sight) coupled with SEM-IT 200 scanning electron microscope (JOEL Corp, Tokyo, Japan) operated at 20 kV of an accelerating voltage for compositional analysis as well as conformation for the presence of elemental zinc.
Transmission electron microscopy. The size and shape of Alk-ZnO NPs were observed using a transmission electron microscope TEM JEM-1400 plus, (JOEL Corp, Tokyo, Japan) operated at an accelerating voltage of 50 kV. A drop of ZnO NPs solution was placed on a carbon coated copper grid followed by water evaporation. The average particles size and the size distribution histogram were determined from microscopic images using a particle size analyzer programe, Image J processing and analysis software (http:// imagej. nih. gov/ ij/ index. html).
Zeta potential measurement. The zeta potential was performed by dispersing 1 mg of ZnO NPs in 10 ml of distilled water followed by sonication for 5 min then measurement using Malvern Zetasizer Nano ZS analyzer (Malvern Instruments, Malvern, UK) 66 .
Fourier transforms infrared spectroscopy. FTIR analysis was done for identification of presumable biomolecules responsible for the reduction of the Zn +2 ions and formation and stability of ZnO NPs. Sample was prepared by mixing Alk-ZnO NPs with potassium bromide KBr using hydraulic press and then dried to remove the moisture content. Infrared spectra were recorded over a range of 450-4000 cm -1 with FTIR spectrophotometer (FTIR spectrum Version 10.5.3, Perkin Elmer).

Conclusions
The present study, built up the first ever account of use of culture supernatant of Alkalibacillus sp. W7 towards extracellular synthesis of zinc oxide nanoparticles. The response surface methodology was applied to optimize the conditions influencing the Alk-ZnO NPs size. The results revealed that the optimization of the reaction parameters was essentially needed and directly affected ZnO NPs size. The fitness of the model was verified and predicted values were confirmed. The synthesized Alk-ZnO NPs with optimized conditions showed maximum absorption peak at 310 nm. The XRD results confirmed the efficiency of the synthesis process, evidencing the production of single crystalline NPs with hexagonal wurtzite structure. The average size of synthesized NPs was 17.5 nm, exhibiting quasi-spherical with smooth surface which was confirmed by TEM and SEM analyses. EDX results confirmed the presence of zinc and oxygen with a pure phase. FTIR analysis clearly showed the formation of ZnO NPs and verified the presence of various biomolecules secreted by Alkalibacillus sp. W7 acting as capping and stabilizing agents. This green synthesis does not need any additive stabilizer which is a positive point in comparison with chemical methods. Our results confirm the potential of Alkalibacillus sp. W7 for ZnO NPs biosynthesis in a simple, fast, cost-effective, convenient and ecofriendly way. Furthermore, the results confirmed that the response surface methodology was beneficial for smaller ZnO NPs size synthesis with great stability over time, and the reaction parameters are directly affecting their size.

Data availability
All data produced during this study are included in this published article.